Dr. Gaurav Acharya PG Resident Department of Orthodontics & Dentofacial Orthopaedics Peoples Dental College and Hospital, Kathmandu Guide- Prof. Dr. Situ Lal Shrestha 1
ORTHODONTICARCHWIRESDr. Gaurav AcharyaPG ResidentDepartment of Orthodontics & Dentofacial OrthopaedicsPeoples Dental College and Hospital, Kathmandu Guide- Prof. Dr. Situ Lal Shrestha
1CONTENTSIntroductionHistoryBasic PropertiesOrthodontic archwires materialsPrecious metalStainless steelCobalt chromium alloysNi Ti alloys22CONTENTSShape and size of different archwiresClinical ImplicationLatest AdvancementSummaryReferences
33INTRODUCTIONActive components of fixed appliances.
Bring about various tooth movements through the medium of brackets and buccal tubes. 4
4HISTORYNoble metals such as Gold, Platinum, Iridium, Silver and their alloys were used.
Had good corrosion resistance, and acceptable esthetics
Lacked the flexibility and tensile strength needed5
HISTORY CONTD..Angle introduced German silver into orthodontics. (1887)
Use prevailed up to 2nd half of the 20th century.
Some of the other materials Angle used were wood, rubber, vulcanite, piano wire and silk thread.
6HISTORY CONTD..In late 1930, stainless steel was introduced for appliance fabrication.
Angle used stainless steel in his last year, as ligature wire.
By 1950s stainless steel alloy was used by most of the orthodontist.
7HISTORY CONTD..Cobalt chrome alloys used as a spring in the watches.
In 1950s cobalt chromium alloys drawn into wires available for use in orthodontic appliances
Marketed as Elgiloy.
8Newer materials due to improvement in metallurgy and organic chemistry8HISTORY CONTD..In 1970s, introduction of titanium alloys as orthodontic wire materials.
Beta titanium alloys were developed around 1980 by Charles J. Burstone, marketed as TMA (titanium-molybdenum alloy).
9HISTORY CONTD..Recent advancement is the introduction of new materials like composites and fibre optics.1010ELASTIC PROPERTIES Elastic behavior defined in terms of stress strain response to an external load
Stress:Internal distribution of loadStrain: Internal distortion produced by the load11Both stress strain refer to the internal state of material being studied.11ELASTIC PROPERTIES CONTD..
Change in lengthOriginal lengthHeighest point where strsss and strain still have the linear relationship. Linear relationship is k/a Hooks Law.12ELASTIC PROPERTIES CONTD..Proportional limitPoint at which any permanent deformation is first observed
13Because some amount of deformation has already occurred.13ELASTIC PROPERTIES CONTD..Yield strengthThe point at which a deformation of 0.1%Wire will not return to the original state after this.
14Because some amount of deformation has already occurred.14ELASTIC PROPERTIES CONTD..Ultimate tensile strengthThe maximum load the wire can sustain
15ultimate strength determines the maximum force the wire can deliver if used as a spring, It is important clinically, especially since yield strength and ultimate strength differ much more for the newer titanium alloys than for steel wires.15ELASTIC PROPERTIES CONTD..Failure Point The point at which the wire breaks.
16ultimate strength determines the maximum force the wire can deliver if used as a spring, It is important clinically, especially since yield strength and ultimate strength differ much more for the newer titanium alloys than for steel wires.16ELASTIC PROPERTIES CONTD..Modulus of elasticity(E)- Ratio between unit stress and unit strain
Measured by the slope of the elastic region.
Describe the relative stiffness or rigidity of the material
17ELASTIC PROPERTIES CONTD..StiffnessProportional to the slope of the linear (or elastic) portion of the curve
More the vertical slope, the stiffer the wire
18ELASTIC PROPERTIES CONTD..RangeDistance that the wire will bend elastically before permanent deformation occurs.
19Along the x-axis to the point at which permanent deformation occurs (yield pt at which 0.1% deformation occurs).
19ELASTIC PROPERTIES CONTD..Springback Ability to undergo large deflections without permanent deformation.
If the wire is deflected beyond its yield strength, it will not return to its original shape, but clinically useful Springback will occur unless the failure point is reached. This springback is measured along the horizontal axis.
20ELASTIC PROPERTIES CONTD..Resilience It represents the energy storage capacity of the wireArea under the stress-strain curve out to the proportional limit.
21ELASTIC PROPERTIES CONTD..Formability Amount of permanent bending the wire will tolerate before it breaks or fails.Area under the curve from yield point to the failure point.22
ELASTIC PROPERTIES CONTD..Flexibility
A flexible material can undergo a large deformation (or large strain) with minimal force, within its elastic limit.
Max. flexibility = Proportional limit Modulus of elasticity23ELASTIC PROPERTIES CONTD..ToughnessForce required to fracture a material.Measured as the total area under the stress strain graph.24ELASTIC PROPERTIES CONTD..Brittleness Considered to be the opposite of toughness. A brittle material, is elastic, but cannot undergo plastic deformation.25ELASTIC PROPERTIES CONTD..Fatigue Repeated cyclic stress of a magnitude below the fracture point of a wire can result in fracture. 26This is called fatigue.
26ELASTIC PROPERTIES CONTD..Requirement of ideal orthodontic wires
High strengthLow stiffnessHigh range High formabilityShould be solderable and weldable so that hooks or stops can be attached to the wire.Reasonable in cost
27In contemporary practice , no archwire meet all these requirements.Best results are obtained by using specific archwires materials for specific purpose.27ELASTIC PROPERTIES CONTD..Effects of geometry of beams
Cantilever beamsBeams supported on only one end.Eg, spring used in the removable appliances like fingerspring
Supported beamsBeams supported on both the ends.Eg, Segment of archwire between two teeth
For analysis orthodontic archwires and springs can be considered as a beams.28ELASTIC PROPERTIES CONTD..Effects of geometry of beams Cantilever beams
For analysis orthodontic archwires and springs can be considered as a beams.29ELASTIC PROPERTIES CONTD..Effects of geometry of beams Supporting beamsStrongerLess springy
Beam is rigidly attached on both endTwice strongOne fourth springy
For this reason, the elastic properties of an archwire are affected by whether it is held tightly or held loosly in the bracket.30ARCHWIRE MATERIALSPrecious Metal Alloy Stainless SteelCobalt- Chromium AlloyNickel Titanium AlloyB- Titanium Alloy
31ARCHWIRE MATERIALSPRECIOUS METAL
Used in the first half of twentieth centuaryGold alloy with platinum, palladium, copper were used.
Because no other material at that time would tolerate the intraoral condition.32ARCHWIRE MATERIALSPRECIOUS METAL
High ductilityInert nature and corrosion resistance - so did not form toxic products with salivaVariable stiffness- by heat treatmentHigh resilience and Ease of soldering33- so could be pulled in to wires of desired33ARCHWIRE MATERIALSPRECIOUS METAL
Elastic force delivery much lessGreater cost compared to other base metal wiresHave minimal use currently34- so could be pulled in to wires of desired34ARCHWIRE MATERIALS CONTD..STAINLESS STEEL
Used for most orthodontic wiresLow cost Excellent formabilityGood mechanical propertiesCan be soldered and welded for the fabrication of complex appliances
35ARCHWIRE MATERIALS CONTD..STAINLESS STEEL
Orthodontic wires are of the 18-8 austenitic type, containing approximately 18% chromium and 8% nickel
36ARCHWIRE MATERIALS CONTD..STAINLESS STEEL
37ARCHWIRE MATERIALS CONTD..STAINLESS STEELResistance to corrosion
The chromium gets oxidizedImpermeable, corrosion resistant layer.(passivation)
38ARCHWIRE MATERIALS CONTD..STAINLESS STEEL
Heated to 400-900 C
Chromium combines with carbon
Corrosion resistance of steel is reduced.
39ARCHWIRES MATERIALS CONTD..COBALT CHROMIUM ALLOYDeveloped during the 1950s as ElgiloyOriginally used for watch springsComposition:Cobalt 40-45%Chromium 15-22%Nickel for strength and ductilityIron, molybdenum, tungsten and titanium to form stable carbides and enhance hardenability.
4040ARCHWIRES MATERIALS CONTD..COBALT CHROMIUM ALLOYSupplied in a softer form
Shaping of wire done in softer form
Heat treatment (500 0C)
Wires get hardened(equivalent to SS)
4141ARCHWIRES MATERIALS CONTD..COBALT CHROMIUM ALLOY
Disappeared by the end of 20th centuaryAdditional costExtra set up for the heat treatment to obtain optimal properties4242ARCHWIRES MATERIALS CONTD..NICKEL TITANIUM ALLOYSUseful during the initial orthodontic alignment.Can apply a light force over a large range of activations.Nitinol (Ni, nickel; Ti, titanium; NOL, Naval Ordnance Laboratory) first Nickel Titanium alloy developed for space program43ARCHWIRES MATERIALS CONTD..NICKEL TITANIUM ALLOYS
Uniquenes in Niti is that the transition between 2 str is fully reversible.In certain transition temperature.Low temp n high stress-M
44ARCHWIRES MATERIALS CONTD..NICKEL TITANIUM ALLOYSShape memoryAbility of material to remember its original shape after being plastically deformed.Certain shape is set at an elevated temperatureWhen the alloy is cooled it can be transitionally deformedHeated enough to regain the austenitic structureOrigional shape is restored
45Ability of the material to remember its original shapeUniquenes in Niti is that the transition between 2 str is fully reversible.Low temp n high stress-M
45ARCHWIRES MATERIALS CONTD..NICKEL TITANIUM ALLOYSShape memorySuperelasticity
Ability of the material to remember its original shapeUniquenes in Niti is that the transition between 2 str is fully reversible.
46ARCHWIRES MATERIALS CONTD..NICKEL TITANIUM ALLOYSSuperelasticityReversible strain wire can withstand due to martensite- austenitic phase transitionTransition to martensitic in response to stress.
47Stress induced martensitic transformation.
47ARCHWIRES MATERIALS CONTD..NICKEL TITANIUM ALLOYSClassification proposed by KusyMartensitic StablisedShow stable martensitic structureNo shape memory and superelasticityMartensitic Active/ ThermoactiveIncreses in temperature change of Austenitic to Martensitic48Stress induced martensitic transformation.
48ARCHWIRES MATERIALS CONTD..NICKEL TITANIUM ALLOYSClassification proposed by Kusy
3. Austenitic ActiveShow pseudoelastic behaviorMartensitic transformation is stress induced
49Stress induced martensitic transformation.
49ARCHWIRES MATERIALS CONTD..BETA- TITANIUM
In orthodontic use about two decades ago by Burstone and Goldberg
The commercial name for this wire is TMA, which represents titanium-molybdenum alloy
50ARCHWIRES MATERIALS CONTD..BETA- TITANIUM
Offers a highly desirable combination of strength, springiness and formability.
Excellent choice for auxiliary springs and for intermediate and finishing archwires
Especially rectangular wires for the late stages of edgewise treatment51ARCHWIRES MATERIALS CONTD..
52ARCHWIRES MATERIALS CONTD..53
SIZE & SHAPEBased on cross section
1. Round 2. Square 3. Rectangular 4. Multistranded
54SIZE & SHAPE CONTD..Shapes of arch wires
Round wiresInitial and intermediate stages of treatment to correct crowding, level the arch, open a bite, and close spaces.
Square or rectangular wiresFinal stages of treatment to position the crown and root in the correct maxillary and mandibular relationship.
55SIZE & SHAPE CONTD..Wire SizeSpecified in thousands of an inch
Eg, .016 inch=16 mil 16 mil 16/4 = 04 0.4 mm40 mil 40/4 = 10 1.0 mm
56SIZE and SHAPE CONTD..57
CLINICAL IMPLICATIONPRINCIPLES IN THE CHOICE OF ARCHWIRES
Move freely within the brackets.At least 2 mil clearance between the archwire and the bracket is needed4 mil clearance is desirableTightly fit rectangular, the position of the root apex could be affected, normally should be avoided.
58For mesiodistal sliding,
4 mil clearance is desirable, and more than that provides no advantage.
58CLINICAL IMPLICATION CONTD..ARCHWIRE FABRICATION
Dental arch form varies among individualsBasic principle - the patient's original arch form should be preserved59Most thoughtful orthodontists have assumed that this would place the teeth in a position of maximum stability, and long-term retention
59CLINICAL IMPLICATION CONTD..ARCHWIRE FABRICATION
Premolar-canine-incisor segment of the arch very nicely for most individuals
For all patients, the fit is not as good
CLINICAL IMPLICATION CONTD..ARCHWIRE FABRICATION
61Brader Arch Form
Based on a trifocal ellipse. The anterior segment closely approximates the anterior segment of a catenary curveGradually constricts posteriorly More closely approximate the normal position of the second and third molars.
CLINICAL IMPLICATION CONTD..WIRE BENDING ROBERTS
Computer-controlled machine to shape the archwire as desired.Reducing the amount of clinical time spent bending archwires 62CLINICAL IMPLICATION CONTD..WIRE BENDING ROBERTSIn lingual orthodontics, the scanned casts needed for fabrication of custom bracket pads provide the data needed to generate computer-fabricated archwires63
CLINICAL IMPLICATION CONTD..WIRE BENDING ROBERTSSuresmile techniqueUses the data acquired via intraoral scan to shape the finishing archwires.64
Intraoral scanning device and its output in the computer screen64CLINICAL IMPLICATION CONTD..WIRE BENDING ROBERTSSuresmile technique65
Wire bending Roberts make the precise bend in the custom archwire.In this system, precise positioning of brackets and special bracketprescriptions are not necessary because the robot can bend the wire asdesired.65CLINICAL IMPLICATION CONTD..WIRE BENDING ROBERTSSuresmile technique66
bends compensating for discrepancies inbracket height and root positioning bends for the maxillary central incisors canbe seen before and after the archwire is tied in.66LATEST ADVANCEMENTBRAIDED AND TWISTED WIRES
Very small diameter SS wire can be braided or twisted together
Comprised of five or seven wrapped around a central wire of same diameter.
Affords extreme flexibility and delivers extremely light forces67
LATEST ADVANCEMENT CONTD..BRAIDED AND TWISTED WIRESAvailable in both round and rectangular shape.
Different type Triple stranded 3 wires twistedCoaxial 5 wires wrapped around a core wire Braded 8 strand rectangular wire.
Used at the beginning of the treatment to align labiolingually displaced or rotated anterior teeth.
LATEST ADVANCEMENT CONTD..Triangular Wire
Triangular in cross-section, .030 inch each side, with rounded edges.In retainers and other removable orthodontic appliances.Various types of clasps made of round wire usually cross the occlusion, creating interferences that can cause patient discomfort.
69LATEST ADVANCEMENT CONTD..Triangular WireThe round wire can act as a wedge to cause inter-proximal spacing, which can disrupt the occlusion, with a potentially adverse effect on long-term stability.Comfort , periodontal health, and appliance stability
LATEST ADVANCEMENT CONTD..Supercable
Comprises seven individual strands that are woven together in a long, gentle spiral Maximize flexibility and minimize force delivery.
LATEST ADVANCEMENT CONTD..Optiflex
Nonmetallic orthodontic arch Got unique mechanical propertiesHighly aesthetic appearance made of clear optical fiber.It comprises of 3 layers.
Silicon dioxide coreSilicon resin middle layerNylon outer layer
LATEST ADVANCEMENT CONTD..Optiflex
A. Silicon dioxide core provides the force for moving tooth.B. Silicon resin middle layer protects the core form moisture and adds strength.C. Strain resistant nylon outer layer that prevents damage to the wire and further increases strength.
LATEST ADVANCEMENT CONTD..Optiflex
Esthetic orthodontic archwire.Stain resistantEffective in moving teeth using light continuous forceVery flexible Can be used with any bracket system
will not stain or loose its clear look even after several weeks in mouth.
74LATEST ADVANCEMENT CONTD..Optiflex
Precuations to be taken:
Should be tied into brackets with elastomeric ligatures.Sharp bends should never be given.Instruments with sharp edges, like the scalers etc should be avoided instead a gentle finger pressure is used to insert the archwire into the slot.75
Metal ligatures should never be usedsince they will fracture the glass core.75LATEST ADVANCEMENT CONTD..Marsenol
Tooth coloured nickel titanium wire . Elastomeric poly tetra fluroethyl emulsion(ETE) coated nickel titanium. Exhibits all the same working characteristics of an uncoated super elastic Nickel titanium wire. The coating adheres, to wire and remains flexible76
LATEST ADVANCEMENT CONTD..Clear polymer archwire
Archwires formed from clear polymersBetter esthetics because the wire can be clear or the same color as the teeth .Physical properties that equal or exceed those of metal archwiresDeveloped using two different approachesa formable and a nonformable alternative.
, so that the wire becomes almostinvisible when used with ceramic brackets77LATEST ADVANCEMENT CONTD..Clear polymer archwire
FormableUsing a polyphenylene polymer. Properties similar to small dimension beta-Ti wires and formability similar to stainless steel wires.Nonformablea polymer resin matrix reinforced with glass fibersA specially modified methacrylate resin serves as the polymer matrix material.78, so that the wire becomes almostinvisible when used with ceramic brackets78LATEST ADVANCEMENT CONTD..Clear polymer archwireAvailable in round and rectangular cross-sectionsCan be paired with esthetic pretorqued and preangulated brackets of the practitioner's choice.Auxiliaries like rotating wedges or bracket repositioning can be used to treat simple cases without custom wires.For more complex cases, a series of preformed custom wires are made using either digital images from scans of dental casts or intraoral scans.
79, so that the wire becomes almostinvisible when used with ceramic brackets79LATEST ADVANCEMENT CONTD..Organic Polymer Wire Retainer(QCM)
Made from 1.6mm diameter round polytheline terephthalate. Used for aesthetic maxillary retainersThis material can be bent with a plier, but will return to its original shape if it is not heattreated for a few seconds at temperature less than 230C(melting point). 80
80LATEST ADVANCEMENT CONTD..Organic Polymer Wire Retainer(QCM)
In prefabricating the QCM retainer wires, the anterior portion of the wire and the wave portion are heat-treated at about 150C immediately after bending.
Patients who have worn aesthetic ceramic or plastic brackets during orthodontic treatment are likely to want aesthetic retainers after treatment.81
LATEST ADVANCEMENT CONTD..Organic Polymer Wire Retainer (QCM)
The new aesthetics organic polymer is easy to fabricate and fit to the dental arch.Easy to fabricate and fit to the dental arch.It requires no special tools or instruments82
LATEST ADVANCEMENT CONTD..Organic Polymer Wire Retainer(QCM)
It consists :Anterior plastic partA flat organic polymer wire with 10 labial torque is attached to 0.032 stainless steel posterior arms, each 11cm long.Plastic portion comes in three intercanine widths, with or without activating omega loops in the posterior arms.
LATEST ADVANCEMENT CONTD..Future of Orthodontic Archwires
Composite materials have been shown in the laboratory to have desirable properties.
Not yet come into clinical use.
Color stability and fluorescence of different orthodontic esthetic archwires by Dayanne Lopes da Silvaa ; Claudia Trindade Mattosb et al. published in Angle Orthodontist, Vol 83, No 1, 2013
To evaluate the color stability of six esthetic archwires at different time periods and their Fluorescence
Samples were evaluated after 7, 14, and 21 days of immersion in staining solution. Color measurements were performed by means of a spectrophotometer
All the esthetic archwires assessed showed noticeable color change after 21 days.
85Galvanic Corrosion Behavior of Orthodontic Archwire Alloys Coupled to Bracket Alloys by Masahiro Iijimaa; Kazuhiko Endob et al. in Angle Orthodontist, Vol 76, No 4, 2006The purpose of this study was to provide a quantitative assessment of galvanic corrosion behavior of orthodontic archwire alloys coupled to orthodontic bracket alloys in 0.9% NaCl solution
Two common bracket alloys, stainless steels and titanium, and four common wire alloys, nickel-titanium (NiTi) alloy, b-titanium (b-Ti) alloy, stainless steel, and cobalt-chromium-nickel alloy, were used.
CONCLUSIONS- Had little effect on galvanic corrosion behavior
86SUMMARYIt is important to know the properties of the archwires as it is widely used in orthodontics.
Proper handling of the material gives the best result.
Materials with excellent aesthetics and strength expected to replace metals in orthodontics in the near future
87ReferencesWilliam R Proffit, Henry Fields, David M Server; Contemporary Orthodontics, 5th editionPhillips science of dental materials, 11th ed, Anusavice Orthodontic Materials, Scientific and Clinical Aspects; William A. Brantley, Theodore EliadesGraber, Vanarsdall, Vig; Orthodontics - Current principles and Techniques88ReferencesColor stability and fluorescence of different orthodontic esthetic archwires by Dayanne Lopes da Silvaa ; Claudia Trindade Mattosb et al. ; Angle Orthodontist, Vol 83, No 1, 2013Galvanic Corrosion Behavior of Orthodontic Archwire Alloys Coupled to Bracket Alloys by Masahiro Iijimaa; Kazuhiko Endob et al.; Angle Orthodontist, Vol 76, No 4, 2006Newer orthodontic wires: A Revolution in orthodontics, Dr. Abhishek Agwarwal, Dr. D. K. Agarwal et al , Orthodontic Cyberjournal, April 2011
89ReferencesClinical comparison and performance perspective of three aligning arch wires, T. Justin W. Evans, Malcolm L. Jones et al; American Journal of Orthodontics and Dentofacial Orthopedics, Volume 114, No. 90